Specific Synthesis of CoS2 Nanoparticles Embedded in Porous Al2O3 Nanosheets for
Efficient Hydrogen Evolution and Enhanced Lithium Storage
Ling Fanga, Yan Zhanga, Yongxin Guana, Huijuan Zhanga, Shilong Wangb*, Yu Wanga*
aThe State Key Laboratory of Mechanical Transmissions and the School of Chemistry and
Chemical Engineering, bCollege of Mechanical Engineering, Chongqing University, 174
Shazheng Street, Shapingba District, Chongqing City, P.R. China, 400044
E-mail: firstname.lastname@example.org; email@example.com
Synthesis of Co6Al2CO3(OH)16∙4H2O nanosheets
All chemicals or materials were utilized directly without any further purification prior to use.
Briefly, concentrated ammonium hydroxide (12.5 mL), ethylene glycol (12.5 mL), Co(NO3)2
aqueous solution (5 mL, 1 M), Al(NO3)3 aqueous solution (2 mL, 1 M), and Na2CO3 aqueous
solution (5 mL, 1 M) were added step by step under strong stirring with intervals of 2 min. After
that, the precursor solution was stirred for another 20 min, and then the mixture changed into
purple solution. Afterwards, the precursor solution was transferred into a Teflon-lined stainless-
steel autoclave with a volume of 50 mL. And thermal treatment was performed on the Teflon liner
in an electric oven at 180 oC for 15 h. After the autoclave was cooled down naturally to room
temperature in air, samples deposited at the bottom of Teflon were collected and washed by
centrifugation for at least three cycles using deionized water and one cycle using pure ethanol. The
as-synthesized samples were then dried in a normal oven at 60 oC overnight to remove the
absorbed water and ethanol for the subsequent fabrication and characterizations.
Synthesis of CoS2 NP/Al2O3 NS
The second step was carried out in a tube furnace to convert the Co6Al2CO3(OH)16∙4H2O
nanosheets into CoS2 NP/Al2O3 NS. Briefly, the graphite boat containing precursor power
(Co6Al2CO3(OH)16∙4H2O nanosheets) were placed in the center of a fused silica tube on a reactor
equipped with both pressure and gas flow controllers. An alumina boat containing 1 g of S powder
(Sigma-Aldrich, 99.5−100.5%) was placed in the tube at the farthest upstream position within the
tube furnace. The tube was purged of air and maintained at 780 Torr under a steady flow of Ar
carrier gas (99.999%) at 25 sccm. The furnace temperature was ramped to 400 °C at a rate of
~10℃ min-1 and held at this temperature for 1 h. After cooling under Ar flow, the samples were
rinsed with CS2 (Sigma-Aldrich, 99.9%) and dried with nitrogen.
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A.
This journal is © The Royal Society of Chemistry 2017
For comparison, bare CoS2 NP was prepared with the same procedure except for adding
ethylene glycol and Al(NO3)3 in the hydrothermal process.
Preparation of pure Al2O3 nanosheets
First, we weighed 300 mg CoS2 NP/Al2O3 NS in 50 mL hot concentrated hydrochloric acid and
stirred for 1 day. After that, the sample was collected by centrifugation and washed with pure
ethanol and D.I. water, and then dried in an oven. The content of Al2O3 in CoS2 NP/Al2O3 NS was
calculated from the formula:
Al2O3% = W(Al2O3)/W(CoS2 NP/Al2O3 NS)*100%
where W(Al2O3) and W(CoS2 NP/Al2O3 NS) are the weight of Al2O3 and CoS2 NP/Al2O3 NS,
A field-emission scanning electron microscope (SEM, JEOL JSM-7800F) coupled with an EDS
analyzer (JEOL, JSM-7800F), TEM coupled with an EDS analyzer (Philips, Tecnai, F30, 300 kV),
X-ray photoelectron spectrometery with a ESCALAB250 analyzer (XPS), powder X-ray
diffraction with Cu Kα radiation (XRD, Bruker D8 Advance), Brunauer-Emmett-Teller surface
area measurement (BET, Quantachrome Autosorb-6B surface area and Pore size analyzer) were
used to characterize the obtained samples.
For HER studies, electrochemical measurement was fulfilled on a CHI660E electrochemistry
work-station, which was conducted in a three-electrode device including a working electrode of
clean glassy carbon electrode (GCE) (0.07 cm2), a reference electrode of saturated calomel
electrode (SCE), and a counter electrode of Pt foil. The catalyst suspension was prepared as
follows: 4 mg of the obtained CoS2 NP/Al2O3 NS composite was dispersed ultrasonically in 100
μL of a diluted Nafion solution (0.5wt %) and 300 μL of ethanol. Then, 4 μL of the suspension
was dropped on the GCE (mass loading 0.57 mg cm−2) and air-dried as working electrode. Linear
sweep voltammetry (LSV) was carried out between -0.2 to -0.6 V at a scanning rate of 5 mV s−1 in
0.5 M H2SO4 solution. The durability analysis was taken by cyclic voltammetry (CV) scanning
from -0.2 to -0.6 V at 50 mV s−1 for 1000 cycles. The stability estimation was taken by
galvanostatic measurement for 10 h at an electrostatic current density of -10 mA cm-2. According
to the equation E(RHE) = E(SCE) + 0.281 V, all the potentials were involved in reversible
hydrogen electrode (RHE) in 0.5 M H2SO4 solution. The onset potential is defined as the potential
at the current density of -1.0 mA cm-2 for HER.
For LIBs test, a homogeneous mixture composed of CoS2 NP/Al2O3 NS, carbon black, and
polyvinyl difluoride (PVDF) using 1-methyl-2-pyrrolidinone (NMP) as solvent in a weight ratio of
70:20:10 was prepared under strong magnetic stirring for at least 1 d. Then some of the mixture
was extracted and spread onto Cu foils. Before and after the samples were spread, the Cu foils
were weighed using a high-precision analytical balance. The read difference was the exact mass
for the coated samples on Cu foils. Normally, the sample loadings range from 1.6 to 1.8 mg·cm-2.
The obtained pieces of Cu covered with samples were then used as working electrodes with 1M
LiPF6 in ethylene carbonate and diethyl carbonate (EC/DMC=1:1 v/v) as electrolyte. Celgard
2400 was applied as the separator film to isolate the two electrodes. Pure Li foil (99.9%, Aldrich)
used as the counter electrode and reference electrode. The cell was assembled in an argon filled
glove box in which moisture and oxygen concentrations were strictly limited to below 0.1 ppm.
The galvanostatic cycling was performed using a Neware battery testing system. The
Electrochemical impedance spectroscopy (EIS) was measured by the CHI604E Electrochemical
Analyzer with the frequency range from 0.01 to 100000 Hz with a sine wave with amplitude of
Fig. S1 The nitrogen absorption/desorption curve of the CoS2 NP/Al2O3 NS and the inset profile
shows the corresponding pore size distribution.
Fig. S2 SEM image of the CoS2 NP/Al2O3 NS after the dissolution of CoS2 nanoparticles in the
hot concentrated hydrochloric acid.
Fig. S3 (a) SEM image and (b) XRD pattern of bare CoS2 NP.
Fig. S4 The polarization curve of the bare Al2O3.
Fig. S5 Nyquist plots of the CoS2 NP/Al2O3 NS and CoS2 NP tested at a given overpotential of 90
mV and the inset shows the equivalent circuit.
Fig. S6 (a) CV curves of the CoS2 NP tested at various scan rates from 5 to 100 mV s-1. (b) The
capacitive currents at 0.225 V vs. RHE as a function of scan rate for CoS2 NP.
Fig. S7 The SEM image of the CoS2 NP/Al2O3 NS after the galvanostatic measurement for 10 h.
Fig. S8 Galvanostatic charge/discharge curves of the bare CoS2 NP at 100 mAh g-1.
Fig. S9 (a) Galvanostatic charge/discharge curves of the bare Al2O3 nanosheets and (b) the SEM
image of the Al2O3 nanosheets after running for 50 cycles.
Fig. S10 SEM image of the CoS2 NP/Al2O3 NS composite after 150 charge/discharge cycles at
100 mA g-1.
Table S1. HER performance of CoS2 NP/Al2O3 NS composite compared with other transition
metal-based catalysts reported in the previous literature.
- 73.4 87
MoS2 nanosheet array/Ti
150 51 225
81 72 193
- 51 142
CoS2-MoS2/CNTs5 70 67 -
CoS2 nano-octahedra on
carbon fibre network
63 73 136
53 50.9 115
* η10: overpotential requirement for current density of 10 mA cm-2.
1. H. C. Zhang, Y. J. Li, T. H. Xu, J. B. Wang, Z. Y. Huo, P. B. Wan and X. M. Sun, J. Mater.
Chem. A, 2015, 3, 15020-15023.
2. Z. Y. Lu, W. Zhu, X. Y. Yu, H. C. Zhang, Y. J. Li, X. M. Sun, X. W. Wang, H. Wang, J. M.
Wang, J. Luo, X. D. Lei and L. Jiang, Adv. Mater., 2014, 26, 2683-2687.
3. H. Zhang, Y. Li, G. Zhang, P. Wan, T. Xu, X. Wu and X. Sun, Electrochim. Acta, 2014, 148,
4. S. J. Peng, L. L. Li, X. P. Han, W.